\begin{figure}
\begin{small}
\beginpicture
\setcoordinatesystem units <1mm,1mm>
\put {~} at -27 0
\tickstovaluesleading10pt
\longticklength4pt
\shortticklength2pt
\setplotarea x from 0 to 90, y from 0 to 60

\axis bottom
        label {$X/\%$}
        ticks in withvalues 0 25 50 75 100 /
        quantity 5 short quantity 9
        /
\axis left
        label {$M_\mathrm{n}/\nicefrac{\mathrm{g}}{\mathrm{mol}}$}
        ticks in withvalues 0 {15\,000} {30\,000} {45\,000} {60\,000} /
        quantity 5 short quantity 9
        /
\axis top
        ticks in quantity 5 short quantity 9
        /
\axis right
        ticks in quantity 5 short quantity 9
        /

\inboundscheckon
\setquadratic
%\setdashpattern <3mm,1mm,0.5mm,1mm>

\plot
0	0.0	
9	5.6	
18	11.2	
27	16.8	
36	22.4	
45	28.0	
54	33.6	
63	39.2	
72	44.8	
81	50.4	
90	56.0		
/

\setdashpattern <3mm,1mm,0.5mm,1mm>

\plot
0	0	
9	8.2	
18	15.8	
27	22.6	
36	28.6	
45	34.0	
54	38.6	
63	42.5	
72	45.7	
81	48.2	
90	49.9			
/

\multiput {$\circ$} at
0.0	0.1	
18.0	19.0	
31.5	25.0	
59.4	40.0	
76.5	46.0	
89.1	51.0	
/

\endpicture

\caption{
Abhängigkeit der mittleren 
Molmasse vom Monomerumsatz für die Polymerisation von {\footnotesize MMA} 
mit {\bf 14} und {\bf 6}
(Reaktionsbedingungen: siehe Tabelle 3.14).
}
\end{small}
\end{figure}
